- Nano Express
- Open Access
Optical absorption and photoluminescence studies of gold nanoparticles deposited on porous silicon
Nanoscale Research Letters volume 8, Article number: 35 (2013)
We present an investigation on a coupled system consists of gold nanoparticles and silicon nanocrystals. Gold nanoparticles (AuNPs) embedded into porous silicon (PSi) were prepared using the electrochemical deposition method. Scanning electron microscope images and energy-dispersive X-ray results indicated that the growth of AuNPs on PSi varies with current density. X-ray diffraction analysis showed the presence of cubic gold phases with crystallite sizes around 40 to 58 nm. Size dependence on the plasmon absorption was studied from nanoparticles with various sizes. Comparison with the reference sample, PSi without AuNP deposition, showed a significant blueshift with decreasing AuNP size which was explained in terms of optical coupling between PSi and AuNPs within the pores featuring localized plasmon resonances.
Coupling system involving semiconductor nanocrystals (NCs) and metal nanoparticles (NPs) has been a subject of great interest for the scientific community . Due to the plasmon resonance in metal NPs, the interplay between NCs and NPs can modify the spectral features of NCs to improve emission efficiency as it involves the charge transfer across the semiconductor/metal interfaces . Gold nanoparticles (AuNPs) are the subject of increasing interests due to their essential properties and localized surface plasmon resonance in the visible spectrum wavelength . The interplay effect in combining the gold and silicon is widely used in electronic devices in controlling their lifetime and resistivity [4, 5].
The AuNPs are mostly fabricated using a combination of chemical e-beam lithography and self-assembly techniques [6, 7] or by electron beam evaporation . However, the challenge is to control the size and position of the nanoparticles because these techniques tend to show a slightly broader size distribution. Mafuné et al.  have developed the laser ablation and laser-induced method to control the size of AuNPs without contamination. Nevertheless, this technique is very costly to implement. As an alternative, electrodeposition technique can offer a solution to the problems as it is known for its simplicity and low processing cost .
Instead of using silicon as the substrate for the AuNP deposition, Fukami et al.  discovered the use of porous Si to control the shape and alignment of metal nanostructures. In this paper, we demonstrate that AuNPs supported on zinc oxide (ZnO) that was synthesized via the deposition-precipitation method can be deposited into porous silicon (PSi) using electrochemical deposition (ECD) technique. The deposition-precipitation method has been proven to produce gold particles of size less than 5 nm . The growth parameters such as pore size distribution of PSi, metal solution concentration, and exposure time may have major influence on the AuNP growth.
Preparation of porous silicon using pulsed technique
An n-type <100 > −oriented silicon wafer with a resistivity of 1 to 10 Ω cm was used to fabricate the PSi substrate. The substrate was cleaned in a wet chemical etching process, using RCA cleaning method. After cleaning, the samples were prepared using pulsed anodic etching method . Output signal from the pulse current generator was used to feed the current at a constant peak of 10 mA/cm2 by adjusting the pause time (Toff) at 4 ms with cycle time Tall (14 ms). The electrolyte solution used was a mixture of hydrofluoric acid and ethanol, 1:4 by volume. Anodization process was carried out for 30 min for all samples under illumination of a 100-W incandescent white light, 15 cm away from the samples. After the etching, the samples were rinsed in deionized water and dried in ambient air.
Preparation of gold nanoparticle supported on zinc oxide
The AuNPs were prepared using the procedure basically similar to that described in our previous work  using deposition-precipitation method. The solution of 100 mL of HAuCl4 solution was heated to 80°C where the pH was adjusted by dropwise mixing with 0.5 M NaOH. Relatively, 1.00 g of zinc oxide support was immersed into the solution. In order to maintain the pH after the support was inserted, dropwise addition of 1.5 M HCl was prepared. The suspension was thermostated at 80°C and underwent vigorous stirring for 2 h. After that, the precipitates were washed with distilled water to remove residual sodium, chloride ions, and unreacted Au species. This process was repeated until there were no AgCl precipitates detected when a filter was added to the AgNO3. The resulting precipitate was gathered by centrifugation and dried at 100°C overnight. The calcination procedure was brought out at 450°C under ambient air for 4 h and a temperature gradient of 50°C min−1. About 0.6 g of black powder was finally obtained. The mean diameter of AuNPs less than 5 nm at pH 7 was obtained.
Fabrication of AuNPs using electrochemical deposition method
The as-prepared Au nanoparticle powder was dispersed in aqua regia  and diluted with deionized water, forming yellow solutions with a mass concentration of approximately 2.8 mg/mL. The aqua regia was prepared by mixing one part of concentrated HNO3 with four parts of concentrated HCL to dissolve the gold. It was stirred using the hot plate magnetic stirrer at 20°C for 15 min. The solvent then was used in electrochemical deposition process using direct current at different current densities of 1.5, 2.5, 3.5, and 4.5 mA/cm2 for 30 min. Gold wire (99.999% purity) was an anode, and PSi was a cathode. The distance between the two electrodes was approximately about 0.5 cm. After that, the samples were dried under nitrogen flow and followed by annealing at 350°C for 15 min. The deposited samples were characterized using scanning electron microscopy (SEM), energy-dispersive X-ray spectroscopy (EDX), X-ray diffraction (XRD), and photoluminescence spectroscopy (PL).
Results and discussion
Transmission electron microscopy
The gold images in the transmission electron microscopy (TEM) analysis (Figure 1) are represented by the small dark particles while the ZnO is shown as the larger particles with less intense color. The TEM images clearly show that the Au particles are deposited on the support. The average size of the Au particles is 4.45 ± 1.80 nm with 1- to 15-nm particle size distribution. It shows that the Au nanoparticles supported on ZnO prepared via the deposition-precipitation method produced average gold particle size less than 5 nm with maximal gold loading.
Scanning electron microscopy
Figure 2a shows the top-view SEM image of the PSi formed using pulsed current method at a constant peak current density of 10 mA/cm2 with cycle time, Tall 14 ms and pulse time, Toff 4 ms. A uniform pore distribution is observed with estimated sizes around 2 ± 1 μm. Average pore depth of about 7.4 ± 3 μm and distinguished sharp pin-shaped holes are observed, as shown in Figure 2b.
Figure 3 shows the SEM images and EDX spectrum of AuNPs deposited on PSi (Au/PSi) at different current densities of 1.5, 2.5, 3.5, and 4.5 mA/cm2 for 30 min. The images showed well-developed, faceted, large Au colloidal crystals prepared through the ECD method. The density of faceted grain sizes of AuNPs changes with current density. The Au colloidal crystal showed a mixture of large and small sizes from 100 nm to 2.0 μm for 1.5 mA/cm2 (Figure 3a), denser and wide distribution of larger grain sizes of Au particles with uniform sizes of 500 nm for 2.5mA/cm2 (Figure 3b), and smaller sizes, denser and more uniform AuNPs having estimated sizes ranging from 100 to 300 nm was observed for 3.5mA/cm2 (Figure 3c). The grain sizes became larger and more widely distributed around the surfaces for 4.5 mA/cm2 (Figure 3d), having homogeneous size distribution around 1.0 μm. The elemental composition of these faceted crystals is qualitatively determined using EDX spectroscopy. The EDX analysis was conducted on the white and black spots, which represent the gold and pores, respectively. The results showed that the significant Au peak appears from the black spot which is the pore area. This suggested that the AuNPs had diffused inside the pore of silicon nanostructures.
The potential reaction observed in dissolving the gold nanoparticle using aqua regia as an electrolyte for the ECD process can be expressed as follows :
This resulted in a removal of positive gold ions (Au3+) from the solution and allowed further oxidation of gold to take place, and so, the gold was dissolved. In addition, Cl− (from hydrochloric acid) removed Au3+ from the solution, encouraging NO3− to dissolve a bit more gold. The longer the process goes on, the larger the Au particles become in size. We believe that there is an appropriate current density in which the formation of a high percentage of Au particle could be accelerated. Accordingly, from the SEM and EDX analyses, when the current density increases from 1.5 to 2.5 mA/cm2, the deposition rate of AuNPs increases. Consequently, at 3.5 mA/cm2, the deposition rate produces Au colloidal crystal with smaller sizes that widely distributed on the substrate. Beyond 3.5 mA/cm2, the deposition rate increases, and it enhances the fabrication of Au grain size. Thus, larger sizes of AuNPs were produced.
Figure 4 shows the typical XRD patterns of Au/PSi at different current densities. The XRD spectrum (Figure 4A) spectrum revealed two peaks: 2θ = 37.7° and 2θ = 38.2° for Si (002) and Au (111). A strong peak at 2θ = 38.2° indicates the higher population of Au (111) , which is the preferred orientation for the gold particle. Among the index facets of Au, Au (111) facet has the lowest surface energy. Thus, during chemical deposition, AuCl4− ions will be preferentially absorbed on other index facets, and these absorbed AuCl4− will be reduced to Au particle by the hydrochloric acid present in the solution. Therefore, the longer the processes go on, the whole substrates become enriched with Au (111) facet and become large in sizes. The XRD patterns of Au embedded into PSi (Figure 4B) revealed the diffraction peaks for cubic gold at 2θ = 64.6°, 77.5°, and 81.7°, which correspond to the crystal planes of (220), (311), and (222), respectively. The strong peak at 2θ = 69.5° is due to Si (422). The estimated Au crystallite size calculated using the Scherrer equation  from this peak is 58 nm for 1.5 mA/cm2, 50 nm for 2.5 mA/cm2, 51 nm for 3.5 mA/cm2, and 40 nm for 4.5 mA/cm2, respectively, indicating smaller crystallite size with increasing deposition current. The current density, angle (2θ), full width at half maximum (FHWM), and Au crystallite size are summarized in Table 1.
Figure 5 shows the PL spectrum of PSi deposited with AuNPs at different current densities. The PL spectrum was characterized by the presence of one sharp peak in the red-band region showing the fundamental absorption of PSi (Eg = 1.91 eV) with the peak centered at 647 nm. It is attributed to the quantum confinement of electrons from Si nanocrystallites . Another emission is observed with energy above the PSi bandgap around 2.34 eV (530 nm) showing broad and intense peak. PL spectrum in this region have different peak positions due to the formation of AuNPs of different sizes. We suggested that the origin of this band comes from the exciting laser that penetrated through the porous layer and directly exciting throughout AuNPs. Optical coupling between them is claimed to govern the observed behavior [19, 20]. Meanwhile, the sample deposited with 3.5 mA/cm2 (sample c) had almost no PL peak that it is not included in the figure. The disappearance of the peak is consistent with the SEM image (Figure 3c) showing that the deposition of AuNPs with smaller grain sizes covered the entire PSi surface, which prevents the optical coupling process from taking place.
AuNPs exhibit the local electric field caused by the localized surface plasmon resonance behavior. When incident laser hits onto the surface, it caused the surface plasmon excitation and locally enhanced the electromagnetic field near the AuNPs and gave rise to PL emission. It has been known that the intensity of the of the plasmon peak is greatly dependent on the size and shape of AuNPs . Therefore, as arranging them in crystallite size, we can see a general trend of increased emitted energy with decreasing crystallite size. Generally, as the gold crystallite size becomes smaller, the PL intensity becomes higher and stronger. Sample d shows the highest PL intensity by a factor of 4 compared to the other samples. It also noted that the plasmon peak exhibits blueshift with decreasing particle size. The observed blueshift in the peak position of plasmon absorption can be attributed to the quantum size effects from the AuNPs . The optical properties of this composite structure, PSi containing AuNPs, reveal dielectric changes when the electromagnetic fields from AuNPs couple with PSi emission that leads to a clear blueshift (relative to the PSi sample) . It is therefore noted that a current density of 4.5 mA/cm2 for electrodeposition produced the highest PL intensity.
In conclusion, we have succeeded growing AuNPs on the surface of PSi using a cost-effective and simple method of electrochemical deposition. We showed that current density of the deposition process defined the size of the formed AuNPs. The surface morphology showed a gold colloidal crystal network with varying sizes. XRD spectra confirmed the element inside the Au/PSi whereby the peaks of Au (111) emerged as the preferred orientation. The samples contain cubic gold phase with crystallite size in the range of 40 to 58 nm. The blueshifted spectrum was caused by the interface interactions between AuNPs and the PSi, which are interpreted in terms of localized surface plasmon resonance of the AuNPs due to the change of the size condition which leads to a spectral shift of the spectrum in the PL.
TSTA is a MSc student of the University Sains Malaysia (USM) together with HY. MRH is professor at the USM. NKA is the senior lecturer at the University Teknologi Malaysia (UTM). RA is an associate professor at USM.
Polisski S, Goller B, Heck SC, Maier SC, Fujii M, Kovalev D: Formation of metal nanoparticles in silicon nanopores: plasmon resonance studies. Appl Phys Lett 2011, 98: 011912. 10.1063/1.3537811
Oskam G, Long JG, Natarajan A, Searson PC: Electrochemical deposition of metals onto silicon. J Phys D: Appl Phys 1927, 1998: 31.
Yavuz MS, Jensen GC, Penaloza DP, Seery TAP, Pendergraph SA, Rusling JF, Sotzing GA: Gold nanoparticles with externally controlled, reversible shifts of local surface plasmon resonance bands. Langmuir 2009, 25: 13120–13124. 10.1021/la901779k
Gösele U, Frank W, Seeger A: Mechanism and kinetics of the diffusion of gold in silicon. Appl Phys Mater Sci Process 1980, 23: 361–368.
Bullis WM: Properties of gold in silicon. Solid State Electron 1966, 9: 143–168. 10.1016/0038-1101(66)90085-2
Zheng J, Zhu Z, Chen H, Liu Z: Nanopatterned assembling of colloidal gold nanoparticles on silicon. Langmuir 2000, 16: 4409–4412. 10.1021/la991332o
Mendes PM, Jacke S, Critchley K, Plaza J, Chen Y, Nikitin K, Palmer RE, Preece JA, Evans SD, Fitzmaurice D: Gold nanoparticle patterning of silicon wafers using chemical e-beam lithography. Langmuir 2004, 20: 3766–3768. 10.1021/la049803g
Sander MS, Tan LS: Nanoparticle arrays on surfaces fabricated using anodic alumina films as templates. Adv Funct Mater 2003, 13: 393–397. 10.1002/adfm.200304290
Mafuné F, Kohno J-y, Takeda Y, Kondow T: Full physical preparation of size-selected gold nanoparticles in solution: laser ablation and laser-induced size control. J Phys Chem B 2002, 106: 7575–7577. 10.1021/jp020577y
Mohanty U: Electrodeposition: a versatile and inexpensive tool for the synthesis of nanoparticles, nanorods, nanowires, and nanoclusters of metals. J Appl Electrochem 2011, 41: 257–270. 10.1007/s10800-010-0234-3
Fukami K, Chourou ML, Miyagawa R, Noval ĂM, Sakka T, Manso-Silvăn M, Martĭn-Palma RJ, Ogata YH: Gold nanostructures for surface-enhanced Raman spectroscopy, prepared by electrodeposition in porous silicon. Materials 2011, 4: 791–800. 10.3390/ma4040791
Yazid H, Adnan R, Hamid SA, Farrukh MA: Synthesis and characterization of gold nanoparticles supported on zinc oxide via the deposition-precipitation method. Turk J Chem 2010, 34: 639–650.
Ali NK, Hashim MR, Abdul Aziz A, Hamammu I: Method of controlling spontaneous emission from porous silicon fabricated using pulsed current etching. Solid State Electron 2008, 52: 249–254. 10.1016/j.sse.2007.08.022
Hutchings G: Catalysis: a golden future. Gold Bulletin 1996, 29: 123–130. 10.1007/BF03214746
Conte M, Carley AF, Heirene C, Willock DJ, Johnston P, Herzing AA, Kiely CJ, Hutchings GJ: Hydrochlorination of acetylene using a supported gold catalyst: a study of the reaction mechanism. J Catal 2007, 250: 231–239. 10.1016/j.jcat.2007.06.018
Chowdhury A-N, Alam MT, Okajima T, Ohsaka T: Fabrication of Au(111) facet enriched electrode on glassy carbon. J Electroanal Chem 2009, 634: 35–41. 10.1016/j.jelechem.2009.07.006
Birkholz M, Fewster PF: High-resolution X-ray diffraction. In Thin Film Analysis by X-Ray Scattering. Berlin: Wiley; 2006:297–341.
Abd Rahim AF, Hashim MR, Ali NK: High sensitivity of palladium on porous silicon MSM photodetector. Physica B: Condens Matter 2011, 406: 1034–1037. 10.1016/j.physb.2010.12.056
Bassu M, Strambini ML, Barillaro G, Fuso F: Light emission from silicon/gold nanoparticle systems. Appl Phys Lett 2011, 97: 143113–143113–143113.
Chan K, Goh BT, Rahman SA, Muhamad MR, Dee CF, Aspanut Z: Annealing effect on the structural and optical properties of embedded Au nanoparticles in silicon suboxide films. Vacuum 2012, 86: 1367–1372. 10.1016/j.vacuum.2012.01.005
Zhou HS, Honma I, Komiyama H, Haus JW: Controlled synthesis and quantum-size effect in gold-coated nanoparticles. Phys Rev B 1994, 50: 12052–12056. 10.1103/PhysRevB.50.12052
Daniel M-C, Astruc D: Gold nanoparticles: assembly, supramolecular chemistry, quantum-size-related properties, and applications toward biology, catalysis, and nanotechnology. Chem Rev 2003, 104: 293–346.
The authors would like to thank the Material Innovations and Nanoelectronics research group (MINE), University Teknologi Malaysia, for their help and support. The authors are grateful for the financial support in part from the Ministry of Science, Technology and Innovation (MOSTI). Support grant from the Research University Grant USM-RU-PGRS grant: 1001/PFIZIK/833030 and Universiti Teknologi Malaysia GUP grants are gratefully acknowledged.
The authors declare that they have no competing interests.
TSTA carried out the main experimental work. MRH supervised the research activity. NKAA organized the manuscript. HY and RA prepared and made the chemical characterization of the AuNPs. All authors read and approved the final manuscript.
About this article
Cite this article
Amran, T.S.T., Hashim, M.R., Al-Obaidi, N.K.A. et al. Optical absorption and photoluminescence studies of gold nanoparticles deposited on porous silicon. Nanoscale Res Lett 8, 35 (2013). https://doi.org/10.1186/1556-276X-8-35
- Gold nanoparticles
- Porous silicon